Test Results Static Test Results A summary of results from static tests for each of the CT and LS specimens is shown in Table 2. Table Summary of the static test data for CT and LS specimens Weld Diameter Max. Strength Material Specimen Type Failure Mode (mm) (Newton) 5765 Interfacial Cross Tension 6210 Interfacial 4.3 Interfacial Lap Shear 13171 Pullout Both-Sides 6555 Pullout Cross Tension 6732 Pullout 5.1 14843 Pullout Both-Sides Lap Shear 15226 Pullout Both-Sides 7253 Pullout Cross Tension 7376 Pullout 5.9 6954 Pullout 17105 Pullout Both-Sides Lap Shear 17020 Pullout 3212 Pullout Cross Tension 3419 Pullout 4.0 4286 Pullout Both-Sides Lap Shear 4447 Pullout 3419 Pullout Tension 3427 Pullout DQSK 4.8 4876 Pullout Both-Sides Lap Shear 5029 Pullout Both-Sides 3941 Pullout Both-Sides Cross Tension 4002 Pullout 5.5 5888 Pullout Both-Sides Lap 5873 Pullout Both-Sides A summary of the results from mixed-mode static tests is shown in Table 3. Table Summary of the static test data for MM specimens Loading Max. Fracture Direction Strength Mode (degrees) (Newton) 9613 Interfacial 0 8747 Interfacial 9345 Interfacial 2445 Interfacial 30 3097 Pull-out 1678 Pull-out 90 1372 Interfacial
Test Results Static Test Results A summary of results from static tests for each of the CT and LS specimens is shown in Table 2. Table Summary of the static test data for CT and LS specimens Material Weld Diameter (mm) Specimen Type Max. Strength (Newton) Failure Mode 4.3 Cross Tension 5765 Interfacial 6210 Interfacial Lap Shear Interfacial 13171 Pullout Both-Sides 5.1 Cross Tension 6555 Pullout 6732 Pullout Lap Shear 14843 Pullout Both-Sides 15226 Pullout Both-Sides 5.9 Cross Tension 7253 Pullout 7376 Pullout 6954 Pullout Lap Shear 17105 Pullout Both-Sides 17020 Pullout DQSK 4.0 Cross Tension 3212 Pullout 3419 Pullout Lap Shear 4286 Pullout Both-Sides 4447 Pullout 4.8 Tension 3419 Pullout 3427 Pullout Lap Shear 4876 Pullout Both-Sides 5029 Pullout Both-Sides 5.5 Cross Tension 3941 Pullout Both-Sides 4002 Pullout Lap 5888 Pullout Both-Sides 5873 Pullout Both-Sides A summary of the results from mixed-mode static tests is shown in Table 3. Table Summary of the static test data for MM specimens Loading Direction (degrees) Max. Strength (Newton) Fracture Mode 0 9613 Interfacial 8747 Interfacial 9345 Interfacial 30 2445 Interfacial 3097 Pull-out 90 1678 Pull-out 1372 Interfacial
Report_v7-intg.docx